Share this document with a friend

4

Transcript

Theory of the Three-Dimensional Quantum Hall Effect in Graphite

B. Andrei Bernevig,1 Taylor L. Hughes,2 Srinivas Raghu,2 and Daniel P. Arovas2,3

1Princeton Center for Theoretical Physics, Princeton University, Princeton, New Jersey 08544, USA2Department of Physics, Stanford University, Stanford, California 94305, USA

3Department of Physics, University of California at San Diego, La Jolla, California 92093, USA(Received 22 February 2007; published 4 October 2007)

We predict the existence of a three-dimensional quantum Hall effect plateau in a graphite crystal subjectto a magnetic field. The plateau has a Hall conductivity quantized at 4e2

@

1c0

with c0 the c-axis latticeconstant. We analyze the three-dimensional Hofstadter problem of a realistic tight-binding Hamiltonianfor graphite, find the gaps in the spectrum, and estimate the critical value of the magnetic field abovewhich the Hall plateau appears. When the Fermi level is in the bulk Landau gap, Hall transport occursthrough the appearance of chiral surface states. We estimate the magnetic field necessary for theappearance of the effect to be 15.4 T for electron carriers and 7.0 T for holes.

DOI: 10.1103/PhysRevLett.99.146804 PACS numbers: 73.43.�f, 71.70.Di

Recent advances in the fabrication of single graphenesheets as well as the striking initial experiments on therelativistic quantum Hall effect in graphene [1,2] havegenerated intense interest in this remarkable material.Most of the theoretical and experimental research hasfocused on the properties of the low energy excitationsclose to half filling which have a Dirac spectrum with aspeed of light of the order of 106 m=s. The spin-unpolarized quantum Hall effect shows a sequence ofplateaus at �xy � �n�

12� � 4 e2

h consistent with the exis-tence of two Dirac cones as well as a spin degeneracy [1,2].

The phenomenon of Hall conductivity quantization is,however, not restricted to two dimensions and can occur inbulk samples, albeit under more stringent conditions. Itwas first observed by Halperin [3] that for a three-dimensional (3D) electron system in a periodic potential,if the Fermi level lies inside an energy gap, the conductiv-ity tensor is necessarily of the form:

�ij �e2

2�h�ijkGk; (1)

where �ijk is the fully antisymmetric tensor and ~G (whichmay be zero) is a reciprocal lattice vector. With the ex-ception of engineered multiquantum well systems [4], thethree-dimensional quantum Hall effect (3DQHE) has beenobserved only in the Bechgaard salts [5,6], where a densitywave forms due to in-plane anisotropy. These materials arehighly 2D, with hopping ratios tx:ty:tz � 1:0:1:0:003. Thec-axis hopping is always neglected.

By contrast, in graphite the effective in-plane nearest-neighbor hopping is tk ’ 3:16 eV and the c-axis hoppingt? ’ �0:39 eV [7]. Indeed, were the graphene sheets ingraphite stacked directly atop one another (����stacking), the dispersion in an external field wouldbe En�B;kz���2t? cos�kzc0�� sgn�n�

�����������������jnjB=B0

ptk, with

B0��hc=e�=3�a20� 7275 T. The c-axis dispersion would

then overwhelm the Landau gaps for fields below B� ��4t?=tk�2B0 � 1800 T, which is unattainably large. This is

typically the scenario in layered materials, even when thehopping anisotropy is as large as 10:1.

In this Letter we show that a true bulk room-temperature3DQHE is realized in doped graphite under a large mag-netic field parallel to the c axis. Three factors conspire torender this possible: the large Landau gap of the integerquantum Hall state in graphene, the weak interplane hop-ping, and especially the Bernal stacking. We first give aphysical argument for the existence of 3DQHE based onadiabatic continuity, then perform a full Hofstadter calcu-lation [8] in 3D of the band and surface state structure,using the realistic Johnson-Dresselhaus [9] Hamiltonianfor graphite, plus a magnetic field. We find the minimummagnetic field necessary for a 3DQHE to be 15.4 T forelectrons and 7.0 T for holes, and show that only one Hallplateau (Fig. 1) will be observed due to band closing in thehigher Landau levels (LLs). Beside the obvious predictionof a plateau in off-diagonal conductive response, we alsopredict that a correlated chiral surface state [10] occurs atthe boundary of the sample. Based on the recent experi-mental focus on graphite [11] we believe our prediction istestable with current experimental techniques. PreviousHall plateaus observed in undoped graphite [12,13] areeven in B and come in multiple sequences consistentwith the graphene QHE plateaus [1,2]. They are hencedifferent than our prediction of a single quantized Hallplateau of Hall conductivity twice as large as the oneobserved in graphene for Fermi level in the first Landaugap of doped graphite.

Graphite is a layered material consisting of weaklycoupled graphene layers in an ���� configuration knownas Bernal stacking [14], as depicted in Fig. 1 [15]. If we‘‘turn off’’ the interlayer hopping, then in a field each layerexhibits a relativistic QHE as previously described, with aLL energy En �

������2np

@v=‘, where ‘ ���������������@c=eB

pis the

magnetic length, n � 0; 1; . . . , and v � 106 m=s. Typicalvalues of the gap are roughly 0.1 eV for B � 10 T and>0:25 eV for B> 40 T, thus making graphene the first

PRL 99, 146804 (2007) P H Y S I C A L R E V I E W L E T T E R S week ending5 OCTOBER 2007

0031-9007=07=99(14)=146804(4) 146804-1 © 2007 The American Physical Society

system to exhibit quantized Hall conductance at roomtemperature. Placing the Fermi level in the first Landaugap, the uncoupled graphene layers trivially exhibit a3DQHE, with the bulk enveloped by a sheath of chiralsurface states as in Fig. 1. Adiabatically reintroducing theintralayer hopping causes almost all the LLs to dispersewith kz. The exceptions are the zero modes, which arestable in an idealized model due to particle-hole symmetry,as we show below. By adiabatic continuity, the sheath ofchiral states (and hence the 3DQHE) must be stable as longas the Landau gap does not collapse.

We first show that the statement above is true for asimplified toy model of graphite. If we introduce a parame-ter x � t?=t

graphite? which interpolates between uncoupled

graphene layers (x � 0) and graphite (x � 1), the minimalHamiltonian of our system is a 4� 4 Hermitian matrixacting on the lattice spinor ( A, B, C, D), where (A, B)and (C, D) are the two inequivalent sites of the lower andupper graphene layers in the Bernal stacking, respectively.Its nonzero independent elements are H AB � �H

�CD ���

3p

2 tka0k�, and H AC � �2t? cos�12 kzc0�. The in-planehopping is tk � 3:16 eV, t? � 0:39 eV is the interlayer(A-C) hopping in graphite (x � 1) [14], and a0 � 2:456 �Ais the graphene lattice constant (in-plane A-A distance).The c-axis lattice constant is c0 � 6:74 �A, and k � kx iky. The in-plane dispersion is expanded about thepoint K � �4�3a0

; 0; 0�, which is the Dirac point in graphene.

In a uniform magnetic field, adopting the gauge ~A �12B��y; x; 0�, the Kohn-Luttinger substitution k ! kx iky �

e@c �Ax iAy� [16]. When x � 1, this is the model

used in [17]. Let by, b be LL creation and annihilationoperators (with b; by� � 1), and introduce the notationcz � cos�12 kzc0�. The Hamiltonian is

H �x� �

0 ��tkb �2t?cz 0��tkby 0 0 0�2t?cz 0 0 ��tkb

y

0 0 ��tkb 0

0BBB@

1CCCA (2)

with � � B=B0. Diagonalizing in the basis � �jni; jn�1i; jni; jn� 1i�, for n > 0, one finds the eigenvalues

En � �n�12��

2t2k� 2t2?c

2z

����������������������������������������������������������������������14�

4t4k� 4�n� 1

2��2t2kt2?c

2z � 4t4?c

4z

q�1=2: (3)

This spectrum has explicit particle-hole symmetry. Forn � 0 there are eigenvalues at ��2t2

k� 4t2?c

2z�

1=2 and adoubly degenerate level at E0 � 0. (All levels receive anadditional double degeneracy owing to the existence of theinequivalent K point.) The next Landau bands are thelowest two energy levels of n � 1. We observe that thegap between the zero mode and the proximate LLs cannotcollapse upon interpolating between x � 0 and x � 1 forany value of the magnetic field. By adiabatic continuity,then, the Hall conductance when the Fermi level is in the3D gap (with doubling for spin) is

�xy �4e2

h

Z d3k

�2��3Im

�@ @kx

��������@ @ky�

� �2n� 1�4e2

h

Z dkz2�� �2n� 1�

4e2

hc0: (4)

With the Fermi level between the zero mode and the firstLL, n � 0 and �xy � 4e2=hc0. The Bernal stacking ofgraphite accounts for the extra factor of 2 relative tographene and

R d2k�2��2 Im h@kx j@ky i � 2n� 1 is the

TKNN integer [18] of the relativistic graphene bandswhen the Fermi level is placed in the nth bulk gap. We

FIG. 1 (color online). (a) Graphite in Bernal stacking.(b) Under strong magnetic field, graphite is gapped in the bulkand exhibits chiral surface sheet states. (c) Idealized Brillouinzone for graphite. (d) Predicted 3D Hall conductivity, quantizedin units of 1=c0. Only one plateau is observable in graphite.

FIG. 2 (color online). Zero mode spectrum and Landau levelsof our toy model in B � 10 T interpolated between graphene(x � 0), with no kz dispersion, and graphite (x � 1). The zeromode (blue line) is doubly degenerate, giving a 3D Hall con-ductance of e2

h1c0

per independent K point per spin.

PRL 99, 146804 (2007) P H Y S I C A L R E V I E W L E T T E R S week ending5 OCTOBER 2007

146804-2

observe that the gap between the first and the second LL ingraphite closes for any realistic value of the B field (Fig. 2),and hence higher n plateaus will not be observed. Zeemansplitting could give rise to a �xy � 0 plateau, but it issmeared by the dispersion of the zero mode in the realisticgraphite model used below, and hence the predicted Hallconductance is sketched in Fig. 1.

The existence of a full gap in the 3D LL spectrum is anartifact of the toy model involving only tk and t?. It derivesfrom the presence of a flat twofold degenerate band at theFermi level along the H-K spines of Brillouin zone[Fig. 1(c)] and the Bernal stacking. More realistic treat-ments, such as the Slonczewski-Weiss-McClure (SWMC)[7] or Johnson-Dresselhaus (JD) [9] models, contain smallc-axis B-B (D-D) hopping terms, through the open hex-agons of the CD (AB) plane. Their value is small on thescale of nearest-neighbor hopping—only 10 meV, leadingto a bandwidth of 40 meV along the H-K spine. But thepresence of such terms is crucial toward understanding theproperties of graphite. At B � 0, they result in semimetal-lic behavior, whereas the toy model incorrectly predicts azero gap semiconductor. For weak fields, they lead tooverlap of the LLs and destruction of the QHE. However,as we shall show, the principal gaps surrounding the centraln � 0 LLs survive for B> 7:0 T (holes) and B> 15:4 T

(particles). Lightly doped graphite, then, will exhibit a3DQHE at these fields. We next describe our solution ofthe JD model in a magnetic field on a torus and a Laughlincylinder, finding the LLs and the surface states, and deter-mining the critical fields Bc at which energy gaps openacross the entire Brillouin zone [19,20].

The JD model [9] is a tight-binding Hamiltonian derivedfrom the k � p theory of SWMC. Its nine parameters aregiven in Table I. In addition to nearest-neighbor hoppings,there are also further-neighbor hoppings, both in-plane(extending to third and fourth neighbor) and betweenplanes. There is also an energy asymmetry � � "A�C� �"B�D�. We introduce a magnetic field via Peierls phases onthe links, preserving all rotational (and screw axis) sym-metries of the lattice, as in Fig. 3.

We solve the model through a combination of exactdiagonalization, Lanczos method (for q > 1000, wherethe flux per hexagonal plaquette is 1=q Dirac quanta �0 �hc=e), and low-field expansion. For the bulk band struc-ture, we impose doubly periodic (i.e., toroidal) boundaryconditions in the (x, y) plane, while to study edge (surface)states we impose singly periodic (i.e., cylindrical) bound-ary conditions. For q > 20 the Hofstadter broadening be-comes negligible and the band energies as a function of kxbecome nondispersive, corresponding to the real situationin which the magnetic field splitting is small compared tothe in-plane hopping amplitude.

TABLE I. Tight-binding parameters

Parameter meV Parameter meV Parameter meV

tk;1AB � tk;1CD 4200 tk;2AB � tk;2CD 512.5 tk;3AB � tk;3CD 15tAC �390 tBD �315 tAD � tBC �44t?AA0 � t?CC0 �19 t?BB0 � t?DD0 10 � 50

FIG. 3 (color online). Hopping matrix elements and flux as-signment. Sites A and B belong to different graphene layers thanC and D. Bernal stacking corresponds to A and C differing by ac-axis translation. Not shown are further-neighbor in-planehoppings tk;2AB and tk;3AB. � � 2�p=q is the magnetic flux perhexagon in units of @c=e, and n runs from 1 to q the size ofthe magnetic unit cell.

FIG. 4 (color online). Clockwise from upper left: (a) B � 5 T,no gap present in the full spectrum. (b) B � 12 T, clear gap inthe hole LL spectrum. (c) B � 20 T clear gaps for both hole andelectron LL. Spin-up (blue line) and spin-down (red line) bandsare shown. (d) Principal energy gaps surrounding n � 0 LLs,including effects due to Zeeman splitting. The particle gapcollapses at Bec � 15:4 T and the hole gap at Bhc � 7:0 T. Allenergies have been shifted upward by 100 meV.

PRL 99, 146804 (2007) P H Y S I C A L R E V I E W L E T T E R S week ending5 OCTOBER 2007

146804-3

We observe the following characteristics of the spec-trum. The zero mode has a dispersion of 40 meV in thelow-field limit. The first LL, however, disperses strongly asa function of kz and for each value of q we scan the energyE�kz� spectrum to look for the smallest gap. Figure 4 showsthe bulk Landau level spectrum for B � 5, 12, and 20 T, aswell as the field dependence of the principal gaps surround-ing the central, weakly dispersive n � 0 LLs. We find thatboth gaps are indirect for B< 30 T. In Fig. 5 we plot thebulk band and surface state spectrum as a function of kxand kz, which proves the existence of gaps and surfacestates over the entire Brillouin zone. On the Laughlincylinder, for each value of kz, we obtain 2 chiral edgestates on each of the upper/lower edges of the cylinder.Unlike the low-field bulk LLs, the edge states disperse as afunction of kx and cross the bulk gap to give a Hallconductivity of 2e2=hc0 per spin, in agreement withthe bulk TKNN analysis. We find that the next gap, inwhich 6e2=hc0 per spin, opens only above B � 1000 T.Thus, only one plateau is observable.

At low fields, each LL accommodates��3p

2 a20B=4�0 �

3:16� 10�6B T� states per carbon atom. Accounting forthe quadruple degeneracy of the LLs (twoK points and twospin polarizations), the central n � 0 levels will be filledfor fields below 20 T at a doping of only 0.025%. For thelowest field for which we predict the effect, the doping is amodest 0.01% which can be achieved by doping withBoron [21]. Unlike in a many-body gap, the Fermi levelis not pinned and the width of the LL will be given by thewidth of the mobility single-particle gap in disordered

graphite. Strong disorder leads to wide Hall plateaus andweak disorder to narrow ones [22].

In addition, the chiral surface sheet should exhibit aballistic, in-plane longitudinal response (�xx ! 0 as T !0) as well as remarkable transport properties along themagnetic field direction [10]. In this direction the systemis a stable metal with a T-independent resistivity �zz,which can be much larger than h=e2. However, unlikeRef. [10] we do expect the metallic phase to be unstableto very strong disorder and impurity concentrations whichlevitate bulk extended states above the Fermi level [23].

B. A. B. wishes to thank F. D. M. Haldane for numerousdiscussions. D. P. A. is grateful to the Condensed MatterTheory group at Stanford University for its hospitality andsabbatical support, and to S.-C. Zhang for discussions.

[1] K. S. Novoselov et al., Nature (London) 438, 197 (2005).[2] Y. Zhang et al., Nature (London) 438, 201 (2005).[3] B. I. Halperin, Jpn. J. Appl. Phys. Suppl. 26, 1913 (1987).[4] H. L. Stormer et al., Phys. Rev. Lett. 56, 85 (1986).[5] L. Balicas et al., Phys. Rev. Lett. 75, 2000 (1995).[6] S. M. McKernan et al., Phys. Rev. Lett. 75, 1630 (1995).[7] J. C. Slonczewski and P. R. Weiss, Phys. Rev. 109, 272

(1958); J. W. McClure, Phys. Rev. 108, 612 (1957).[8] D. R. Hofstadter, Phys. Rev. B 14, 2239 (1976).[9] L. G. Johnson and G. Dresselhaus, Phys. Rev. B 7, 2275

(1973); S. Y. Leung and G. Dresselhaus, Phys. Rev. B 24,3490 (1981).

[10] L. Balents and M. P. A. Fisher, Phys. Rev. Lett. 76, 2782(1996).

[11] S. Y. Zhou et al., Nature Phys. 2, 595 (2006).[12] H. Kempa, P. Esquinazi, and Y. Kopelevich, Solid State

Commun. 138, 118 (2006).[13] Y. Kopelevich et al., Phys. Rev. Lett. 90, 156402 (2003).[14] M. S. Dresselhaus and G. Dresselhaus, Adv. Phys. 51, 1

(2002).[15] We have found that 3DQHE exists in rhombohedral

graphite as well, which has ABCABC stacking (detailsto be presented in a future publication).

[16] J. W. McClure, Phys. Rev. 119, 606 (1960).[17] J. Nilsson, A. H. Castro Neto, F. Guinea, and N. M. R.

Peres, Phys. Rev. Lett. 97, 266801 (2006).[18] D. J. Thouless, M. Kohmoto, M. P. Nightingale, and M.

den Nijs, Phys. Rev. Lett. 49, 405 (1982).[19] Earlier calculations for graphite in a large B field, as in

Refs. [16,20], did not address the 3DQHE, nor edge states,and generally neglect the parameter tBD, which we findhas a significant effect on the critical fields.

[20] Y. Iye et al., Phys. Rev. B 25, 5478 (1982).[21] Y. Hishiyama et al., J. Mater. Res. 17, 75 (2002).[22] J. T. Chalker and A. Dohmen, Phys. Rev. Lett. 75, 4496

(1995).[23] R. B. Laughlin, Phys. Rev. Lett. 52, 2304 (1984).

FIG. 5 (color online). Zero mode, first electron Landau level,and surface state spectrum over the first Brillouin zone for onespin species at B � 40 T. (a) Surface state spectrum, (b) surfacestate and bulk n � 0; 1 Landau levels where the n � 1�n � 0�levels are shifted by �0:1 eV ��0:1 eV� for clarity. (Inset) n �0; 1 Landau levels unshifted without surface states.

PRL 99, 146804 (2007) P H Y S I C A L R E V I E W L E T T E R S week ending5 OCTOBER 2007

146804-4

Recommended